CORROSION INHIBITION OF WET GAS PIPELINES UNDER HIGH GAS AND LIQUID VELOCITIES
Michael Swidzinski Phillips Petroleum 35 Guildford Road, Woking Surrey GU22 7QT, UK Bob Fu and Audrey Taggart Nalco/Exxon Energy Chemicals, L.P.7705 Highway 90-A Sugar Land, Texas 77478, USA
W. Paul Jepson Corrosion in Multiphase Systems Center Department of Chemical Engineering, Ohio University Athens, OH 45701, USA
ABSTRACT Work was conducted to assess the applicability of carbon steel pipeline and corrosion inhibitor as a viable combination for transporting wet multiphase corrosive petroleum fluids under high gas and liquid velocities. Flow loop tests were performed to study the performance of inhibitors under simulated field conditions with gas and liquid velocity as high as 25 rn/s. The results showed that inhibition efficiency greater than 96% can be achieved with 100 to 200 ppm of corrosion inhibitors specially formulated for high shear applications. The performance of inhibitors with respect to concentration showed a typical profile similar to that observed at lower velocity. The effective concentration was dependent upon the flow regime. Slug flow typically required a higher concentration due to its severe flowing condition. The positive results support the combined use of carbon steel and corrosion inhibition as a viable and cost-effective option for the development of a pipeline system for the transportation of wet corrosive multiphase hydrocarbon fluids at high velocity.Keywords: wet gas, CO2 corrosion, high velocity, corrosion inhibition, and [email protected] by NACE International.Requests for permission to publish this manuscript in any form, in part or in whole must be in writing to NACE International, Conferences Division, P,O. Box 218340, Houston, Texas 77218-8340. The material presented and the views expressed in this paper a r e solely those of the author(s) and are not necessarily endorsed by the Association. Printed in U.S.A.
INTRODUCTION As more and more energy reserves have been discovered in remote areas, such as in deepwater offshore, it has become increasingly challenging to efficiently produce the petroleum fluids from these remote locations. One major challenge is to transport these "unprocessed", multiphase fluids from the remote area to the central processing facility safely and cost effectively. In order to assure an uninterrupted flow of fluids, or ultimately the flow of revenues, the operator must inhibit any deposition of solids, such as scales, hydrates, waxes and asphaltenes, while maintaining the integrity of the production system by minimizing corrosion and/or erosion. This paper is to address the issues related to corrosion and inhibition of pipelines carrying high velocity gas or liquids. Carbon dioxide corrosion in wet gas pipelines is a well-known phenomenon. 1-4 Extensive studies have been carried out in order to better understand the corrosion mechanisms. 57 These studies were often conducted in laboratories where a much smaller scale system, such as high-pressure flow loops, was built to simulate the real life system. 81 A number of test protocols have also been developed for these simulation systems. The resulting experience had contributed to significant improvement in corrosion control and mitigation for the past two decades. These laboratory scale systems not only were used to assess the severity of corrosion, quite often they were also used as the screening tools for selection of corrosion inhibitors, t0-15 In the production and transportation of petroleum fluids from remote locations, multiphase flow is often encountered and a range of different flow regimes can be experienced in pipelines. For example, the flow regimes can be stratified, slug or annular in horizontal and slightly inclined pipelines. The predominant flow regime is determined by the flow rates and gas/liquid ratio. The wall shear stress associated with these flow regimes, particularly slug flow, is very different from those in the singlephase flow. 5 Despite the advances in the past few decades, the effect of flow on corrosion is not completely understood, especially when multiphase flow is involved. 16-18 Most laboratory tests have been carried out in small diameter (< 5 cm) single-phase flow systems using actual or synthetic fluids. The effect of wall shear stress in these systems shows a general trend of increasing corrosion rate with increasing liquid velocity and hence increasing shear stress. Inhibitors have been shown to provide good corrosion protection in these systems, which can generate shear stress as high as 300 Pa. However, study of corrosion in multiphase flows requires a more sophisticated multiphase flow simulator. A much higher shear stress can be generated in slug flow due to tremendous turbulence at the front of the slug. At slug front gas bubbles are entrained in the liquid and forced towards the bottom of the pipe where they impact and sometimes collapse on the wall, resulting in instantaneous high shear on the wall. Values as high as 3000 Pa have been recorded in the authors' laboratory. 1 When evaluating corrosion inhibitors, it is important to consider all of these flow effects that might exist in the multiphase pipelines. This work was initiated to assess the viability of using the combination of carbon steel and corrosion inhibitor as the design base for the construction of a multiphase pipeline. The pipeline will be used to transport wet gas from a new development located in the North Sea. The diameter of the pipeline must be carefully sized in order to achieve the maximum throughput without causing excessive corrosion and erosion resulting from high fluid velocities. Higher throughput is preferred because of the t The values were recordedwhen the slugs were passingby the hot film probe.
advantage of having higher production rates and lower liquid holdups. However, higher fluid velocity generates higher wall shear stress that can be detrimental to the inhibitor film on the surface. It is believed that there exists a velocity limit above which the inhibitor film is likely be stripped from the surface. 2z2 The challenge to the design engineers is to find the optimum pipeline dimension that offers the highest throughput while keeps the fluid velocity below the safe limit. The inhibitor film remains stable on the surface under this limit. In this study, the corrosiveness of petroleum fluids under selected, severe flowing conditions was established and the ability of inhibitors to mitigate the flow enhanced corrosion was investigated Two corrosion inhibitors, A and B, that have been specifically formulated for high velocity applications were evaluated in this study. Inhibitor A is a polyamidoamine-based formulation and inhibitor B is an imidazoline-based blend. The work was carried out in two high-pressure flow loops, one single-phase and the other multiphase. The single-phase flow loop was used for the study of high liquid velocity and the geometrical effect. The multiphase flow loop was used to study high gas velocities and the flow regime effect.
Single-phase Flow Loop Study The single-phase flow loop used in this study is a 2.54-mm closed loop that has three parallel test sections. The schematic of this loop is shown in FIGURE 1. The details of this loop and its operation are published elsewhere. 9 The test specimens were machined from a pipe section of API X-65 grade. Specimens of two different shapes were used in the experiments. The ring-type specimens (dimension: 6.4 mm ID x 9.5 mm length) were used for the flow-through probe. The tube-shape specimens (dimension: 5 mm OD x 45 mm length) were used for the elbow and dead leg probes. The surface-to-volume ratio was about 1 cm 2 metal surface per 1075 cm 3 fluid. Prior to each test, the specimens were pre-conditioned by being sandblasted with 60-100 mesh amorphous glass beads. The specimens were then sonically cleaned in acetone, rinsed with isopropanol, dried and weighed, before being mounted on the probe. A total of three probes, each mounted in a different geometrical location, were used in each test. Corrosion rates were measured using LPR (linear polarization resistance) technique as well as weight loss method. Following each test, the specimens were removed, dried, and immersed in an inhibited acid for 5 minutes. The inhibited acid was a 2:2:1 mixture of acid:water:commercial corrosion inhibitor. The electrodes were then removed, cleaned with soap and steel wool, and dried. Isopropanol was then used to rinse off any organic residues before the electrodes were weighed for weight loss measurement. The test fluid consisted of the synthetic brine and a hydrocarbon solvent (a hydrotreated light paraffinic distillate). The brine to hydrocarbon ratio was 9:1. The liquid velocity ranged from 2 to 14 m/sec. The temperature and pressure were fixed at 93C and 0.8 MPa, respectively. The flow loop was under a CO2 blanket throughout the test to simulate the sweet condition. The oxygen content was measured after each test to be less than 5 ppb. The composition of the synthetic brine, listed in TABLE 1, was based on the water analysis from a test well.
TABLE 1. The composition of the synthetic brine used in the flow loop study Ionic Species Concentration, ppm Na5 49,047Ca 2+ Mg 2+
Ba z+ 230
Sr2+ HCO3" ,800 , 245
IAnnular f/ow-thru probes .............. i
lOG AutoLm J dead-leg
FIGURE 1. The schematic diagram of the high pressure single-phase flow loop
Multiphase Flow Loop Study The multiphase flow loop is a 10.2-mm high-pressure loop that can be operated at pressure up to 17.2 MPa and te